Yi, J. et al. (2013). Graphite-anchored lithium vanadium oxide as anode of lithium ion battery. Elecrochimica Acta, 106: 534-540
University of the Western Cape Research Repository email@example.com Graphite-anchored lithium vanadium oxide as anode of lithium ion battery
Jin Yi, Julian Key, Fei Wang, Yonggang Wang, Congxiao Wang and Yongyao Xia Abstract
Graphite-anchored lithium vanadium oxide (Li1.1 V0.9 O2 ) has been synthesized via a “one-pot” in situ method. The effects of the synthesis conditions, such as the ratio of reaction components and calcination temperature, on the electrochemical performance are systematically investigated by means of scanning electron microscopy (SEM), X-ray diffraction (XRD), electrochemical impedance spectroscopy (EIS), galvanostatic discharge/charge tests and differential scanning calorimetry (DSC). Compared with the simple mixture of graphite and lithium vanadium oxide, the graphite-anchored lithium vanadium oxide delivers an enhanced reversible capacity, rate capability and cyclic stability. It also shows better thermal stability.
With recent advances in electronic devices, anode materials with high storage capacity and high power density attract considerable interest as alternatives to the
commercial graphite anode used in lithium ion batteries [1,2]. The layered
structured lithium vanadium oxide (Li1.1V0.9O2), has a low working potential of approximately 0.1 V vs. Li+/Li, with a gram speciﬁc capacity of, (314 mAh/g) similar to graphite (372 mAh/g), but shows a higher volumetric capacity density of 1360 mAh/cm3 (790 mAh/cm3 for graphite), and is therefore of considerable
interest as an anode material [3,4]. However, its use is inhibited by its large
volume expansion during Li intercalation, which causes particle fracture and a
subsequent decay of capacity .
Due to the similar lithium intercalation voltage of graphite and lithium vanadium oxide, the two materials are usually mechanically mixed to form a mixture anode that has a higher volumetric energy density than pure graphite and better cyclic
performance than pure lithium vanadium oxide . However, the mixture still
lacks sufﬁcient reversible capacity and cyclic performance, most likely due to a loss of contact between the graphite and lithium vanadium oxide during cycling. In this work, we reported a graphite-anchored lithium vanadium oxide complex (GA-LVO) synthesized using a “one-pot” in situ method to improve the contact between the graphite and lithium vanadium oxide. The effects of the synthesis conditions, including the ratio of reaction components and calcination temperature,
on the electrochemical performance of the GA-LVO were investigated. Carbon-coating technology was applied to enhance the reversible capacity and cycling stability.
2.1 Chemicals and synthesis
Graphite-anchored lithium vanadium oxide (GA-LVO) was synthesized by mixing V2O3 (Aldrich, 98%) and Li2CO3 (Alfa Aesar, 99.99%) in a molar ratio of 1.1: 0.9 (Li to V) with natural graphite (Superhoo Co., Ltd., Yunan). The mixtures were ball-milled in a planetary ball mill at 350 rpm for 6 h under argon protection. The ball-milled powders were then sintered at 850 ◦C or 1100 ◦C for 12 h under ﬂowing Ar gas containing 5% (v/v) H2 and cooled to room temperature. A series of GA-LVO samples with different ratios of LVO to graphite were prepared by the same synthesis processes. For comparison, pure Li1.1V0.9O2 (P-LVO) was synthesized under the same conditions without graphite addition.
A carbon coated GA-LVO (C-GA-LVO-1) sample was prepared by the following process: 4 g GA-LVO-1 powder (see above) was added to a 100 ml ethanol solution containing 10 wt% sucrose (relative to the GA-LVO-1 powder) and stirred for 1 h. The mixture was dried at 80 ◦C for 24 h. The dried powder was ground, sintered at 750 ◦C for 10 h
under ﬂowing Ar gas containing 5% (v/v) H2, room temperature.
For comparison, a mixture of P-LVO and natural graphite (MG-LVO) was prepared by the ball-milling process in a planetary ball mill at 350 rpm for 6 h under argon
protection. The preparation conditions for all samples are summarized in Table 1.
The particle size and morphology were characterized using a JEOL JSM6390 scanning electron microscope (SEM). X-ray powder diffraction (XRD) patterns were recorded on a Bruker D8 X-ray diffractometer at a scan rate of 0.02 ◦ s−1
using Cu Ka radiation (, = 1.5406 A˚ ).
The working electrodes were prepared by mixing 90% of the sample powders, 5% carbon black and 5% polyvinylidene ﬂuoride (PVDF) dissolved in N-methyl-pyrrolidone (NMP), and the slurries were coated on copper foil using the doctor–
blade technique. The electrode ﬁlms were dried at 80 ◦C for 2 h to remove the solvent before pressing. The electrode ﬁlm was punched in the form of disks, typically with a diameter of 12 mm, and then dried at 80 ◦C for 12 h under vacuum. The typical mass loading of the active material of the working electrodes was approximately 5 mg. Electrochemical tests were conducted using CR2016-type coin cells. The cells were assembled with the working electrode as prepared, lithium metal as anode, and Celgard 2300 ﬁlm as separator in a glove-box ﬁlled with pure argon. The electrolyte solution was 1 M LiPF6 dissolved in ethylene carbonate (EC)/dimethyl carbonate (DMC)/diethyl carbonate (DEC) (1:1:1 by volume). Galvanostatic discharge/charge experiments were performed between 2.5 and 0.0 V at various constant current rates on a LAND CT2001A Battery Cycler (Wuhan, China). Lithium insertion into the working electrode was referred to as discharge, and the extraction as charge. The cell capacity was calculated based on the pure weight of active material.
Electrochemical impedance spectroscopy (EIS) was conducted in a three-electrode cell, in which lithium metal was used as both the counter and reference electrodes. The cells prepared as above were left to stand for several hours to equilibrate (SOC = 0) before EIS measurements. The experiments were carried on a Solartron Instrument Model 1287 electrochemical interface and 1255B frequency response analyzer controlled by a computer. The frequency limits were set at 105–10−2 Hz with an ac oscillation of 5 mV. The EIS results were simulated by using ZPVIEW software.
2.4. Thermal stability tests
Electrode materials for differential scanning calorimetry (DSC) measurements were carried as follows. The cells were ﬁrst discharged to a fully lithiated state and disassembled in a glove-box, then the obtained electrodes were dipped into DMC to remove residual LiPF6, Approximately 3 mg of the electrode materials were scraped from the copper current-collector.
The obtained materials were hermetically sealed in gold-plated copper stainless steel capsules in the glove-box. The solid to electrolyte ratio was ﬁxed at 1:2
(w/w) to ensure the presence of excess electrolyte during the experiments. The DSC scans were performed using a DSC 200 F3 instrument (NETZSCH, Germany) with a scanning rate of 10 ◦C min−1. The masses of the DSC pans were measured before and after the DSC measurements to ensure that no leakage
occurred during the experiments .
3. Results and discussion
The effect of synthesis temperature on the phase composition of the samples was ﬁrstly examined. In the previous studies, the P-LVO was prepared at 850 and
1100◦C [3,4]. Therefore, both GA-LVO-1 and P-LVO were prepared at 850◦C. The
XRD pattern of P-LVO (Fig. 1a) prepared at 850 ◦C was indexed to a hexagonal
structure with the R-3m space group, which is consistent with the previously
reported results . When graphite was added at 850 ◦C, the diffraction line
ascribed to Li1.1V0.9O2, and graphite became visible (Fig. 1b), indicating that the
presence of graphite did not affect the synthesis of the Li1.1V0.9O2 at 850 ◦C. However, the XRD pattern for GA-LVO-1100 (from the sample synthesized at
1100 ◦C) (Fig. 1c) notably lacks the characteristic diffraction line ascribed to
Li1.1V0.9O2 prepared at 1100 ◦C that was observable in previous reports . The
XRD instead shows a pattern characteristic of V8C7 (PDF: 35-0786), i.e., a
reaction product of V2O3 and C under high temperature , which occurs via the
4V2O3(s) + 19C(s) = V8C7(s) + 12CO(g) ↑
Therefore, the preparation temperature of 850 ◦C was used in the following experiments.
Fig. 2 shows the morphologies of P-LVO synthesized without adding graphite,
GA-LVO-1 synthesized via the in situ synthesis strategy at 850 ◦C and MG-LVO prepared
by ball-milling P-LVO and graphite together. The SEM images in Fig. 2a and b show
that the Li1.1V0.9O2 particles have a uniform size of approximately 1 µm diameter
and agglomerate into clusters. Fig. 2c and d shows that in the GA-LVO-1 sample,
Li1.1V0.9O2 is anchored to the surface of graphite, which may achieve in the process of the melt of Li2CO3 following the reaction with V2O3. Whereas in the
MG-LVO (Fig. 2e and f), the separated particles of Li1.1V0.9O2 and graphite are
clearly observed. These results indicate that the in situ synthesis strategy prevented the agglomeration of Li1.1V0.9O2 and improved the contact between Li1.1V0.9O2 and graphite, which should lead to the improved electrochemical performance.
Fig. 3A and B show the ﬁrst three discharge/charge curves of GA-LVO-1 and
MG-LVO at the rate of 0.1 C. The discharge capacity was 306 mAh/g for GA-MG-LVO-1, with a reversible efﬁciency of 79%. For comparison, the discharge capacity of the composite MG-LVO (prepared by ball-milling P-LVO and graphite at a 1:1 mass ratio) was 346 mAh/g at 0.1 C, with a reversible efﬁciency of 72%. Compared with GA-LVO-1, the lower reversible efﬁciency of MG-LVO may be due to the larger Li consumption on the formation of the solid electrolyte interface (SEI) and side reactions on the
surface of the electrode. Fig. 3C shows the ﬁrst three discharge/charge curves P-LVO,
where the discharge and charge capacities of P-LVO were 309 and 192 mAh/g,
respectively (the theoretical speciﬁc capacity of Li1.1V0.9O2 is 314 mAh/g ). The
large irreversible capacity may have been caused by the following: (i) Li being trapped in a layered structure of Li1.1V0.9O2, (ii) Li consumption in the formation
of SEI, and (iii) side reactions on the surface of the electrode, such as the
reduction of electrolyte and contaminant (H2O and O2) . GA-LVO-1 showed
better cycling stability compared with MG-LVO. The charge capacity of GA-LVO-1 was
232 mAh/g after 50 cycles at 0.1 C (shown in Fig. 3D), with a corresponding capacity
retentions of 96%, whereas the charge capacity was 208 mAh/g for MG-LVO, with a corresponding capacity retention rate of 83%. However, a sharp decay in the charge capacity for MG-LVO occurred before the tenth cycle, which is mainly attributed to
volume change and the two-phase nature of the intercalation reaction . Similar
results were obtained for P-LVO (shown in Fig. 3D). The phenomenon of sharp
decay was alleviated after the lithium vanadium oxide was anchored on the surface of the graphite, because graphite provides a support for the small particles derived from the electrochemical grinding with high electrical conductivity and enhances Li ion diffusion as well as capacity utilization. Consequently, the graphite-anchored lithium vanadium oxide prepared through the “one-pot” in situ synthesis strategy displayed the improved reversible capacity and cyclic performance.
The rate performance of GA-LVO-1 and MG-LVO is shown in Fig. 4. The charge
capacity for GA-LVO-1 was 219 mAh/g at 0.2 C and 191 mAh/g at 0.5 C, while 194 and 136 mAh/g for MG-LVO, respectively. Compared with MG-LVO, the larger reversible capacity and superior cyclic performance of GA-LVO-1 may stem from the uniform distribution and anchoring of Li1.1V0.9O2
In contrast to Li1.1V0.9O2 agglomeration, the graphite-anchored lithium vanadium oxide increased the contact with graphite. Simultaneously, small particles created by the electrochemical grinding during cycling are supported on the surface of graphite and may enhance the rate capability and cyclic performance
The graphite-anchored Li1.1V0.9O2 provides the support for Li1.1V0.9O2 during cycling, which is an important factor for improving electronic conductivity, cyclic and rate performance. Electronic conductivity and electrochemical
resistance can be determined by electrochemical impedance measurements .
Fig. 5 shows the electrochemical impedance spectra of the prepared samples at
open circuit potentials and the corresponding equivalent circuit. In the equivalent
circuit, Rs is the ohmic resistance of the electrolyte and current collector, Cdl Li+,
is the double-layer capacitance, and Rct is the charge-transfer resistance at the
bulk-electrolyte interface. ZW relates to Li+ diffusion in the inserted materials, and
Cint Li+ relates to the insertion capacitance, reﬂecting the occupation of Li+in the
inserted sites [11–13]. Fig. 5 shows that the experimental data (dots) ﬁtted well
with the equivalent circuit (the solid lines represent the ﬁtted results). The
resistance (Rct) (obtained by ﬁtting the equivalent circuit), which determines the
charge transfer process of the lithium ion insertion/extraction reaction, is 20.7 and 23 Q for the GA-LVO-1 and MG-LVO, respectively. Compared with MG-LVO, the lower resistance conﬁrms that the graphite-anchored lithium vanadium oxide has low charge-transfer resistance, which accounts for better reversible capacity and cyclic performance as anode of lithium ion battery.
The effect of the graphite content ratio to LVO (graphite: LVO) on the speciﬁc capacity and cycling performance of GA-LVO was also investigated.
The calculated mass and volumetric capacity, reversible capacity and initial
coulombic efﬁciency are summarized in Table 2. The cyclic performance of the three
samples is shown in Fig. 6A. The charge capacity after 50 cycles was 96 mAh/g for
GA-LVO-0.5, 232 mAh/g for GA-LVO-1 and 279 mAh/g for GA-LVO-2, corresponding
to capacity retentions of 54%, 96% and 96%. Fig. 6B gives the rate capability of all
three samples. At 0.2 C, the charge capacity was 82, 219 and 266 mAh/g for GA-LVO-0.5, GA-LVO-1 and GA-LVO-2, respectively. When the current rate was raised to 0.5 C, the charge capacity reduces into 29, 192 and 234 mAh/g. All above ﬁnding indicates that the more content of the graphite content will have better reversible capacity and cyclic stability. As a ﬁnal goal to obtain a high volumetric energy density electrode, LVO content should be adopted as high as possible, but this will reduce its cycling stability. Considering both the volumetric capacity and cycling stability, a mass ratio of graphite to LVO of 1:1 is selected.
Controlling the problem of thermal runaway in cells is vital for the commercial use of
lithium ion batteries [14–16]. The DSC curves of the GA-LVO-1 and MG-LVO
electrodes at a fully lithiated state are shown in Fig. 7. The exothermic peak at 104
and 135 ◦C for MG-LVO and GA-LVO-1 is due to the initial SEI ﬁlm decomposition, and the lower exothermic peak and larger heat generation for MG-LVO compared with GA-LVO-1 is caused by the larger SEI ﬁlm decomposition, which would account for the larger initial irreversible efﬁciency of 28% for MG-LVO compared with 21%
for GA-LVO-1 [14,17]. A mild heat ﬂow generation continued from 135 ◦C until a
sharp exothermic peak appeared at 280 ◦C for both samples comes from the reaction
of lithiated graphite with the electrolyte to form a new SEI .
Meanwhile, a sharp exothermic peak was detected at 315 and 323 ◦C for MG-LVO and GA-LVO-1, respectively, which is attributed to the graphite structural collapse
reaction between the graphite and the electrolyte .
From the above DSC results, compared with MG-LVO, the thermal stability of graphite-anchored lithium vanadium oxide has been improved with acceptable thermal stability for application as an anode material for lithium ion batteries. Carbon coating is an important technology used to improve the electrochemical performance of electrode materials in lithium ion batteries. In this study, carbon coating was used to improve the reversible capacity and rate capability of
GA-LVO-1. Fig. 8A shows that C-GA-LVO-1 had a high initial charge capacity of 290
mAh/g with a reversible efﬁciency of 70%. Compared with GA-LVO-1, thelarger irreversible efﬁciency may be due to larger Li consumption in the formation of the
SEI after carbon coating. Fig. 8B shows the cycling stability performance of
C-GA-LVO-1 after 50 cycles at 0.1 C. The charge capacity of C-GA-C-GA-LVO-1 was 282 mAh/g, with negligible capacity decay. The rate capability performance improved after
using the carbon-coating technology (shown in Fig. 8C). At 0.2 and 0.5 C, the
charge capacity was 274 and 260 mAh/g. Compared with GA-LVO-1, the reversible capacity and rate capability at different rates were remarkable improved by increasing the electrical conductivity and enhancing the contact between Li1.1V0.9O2 and graphite after carbon coating.
Graphite-anchored lithium vanadium oxide was successfully synthesized via a “one-pot” in situ method at an optimal synthesis temperature of 850 ◦C. Synthesis at 1100 ◦C produced the by-product V8C7. The graphite-anchored lithium vanadium oxide had lower electrochemical resistance and better thermal stability than the composite prepared by mixing graphite and lithium vanadium oxide, which resulted in a larger reversible capacity, better cycling. Moreover, the carbon coated composite showed the signiﬁcantly improved electrochemical performance with a reversible capacity of 282 mAh/g and negligible capacity decay after 50 cycles. The graphite-anchored lithium vanadium oxide described in the present work is an attractive candidate for anode material in lithium ion batteries.
This work was partially supported by the State Key Basic Research Program of PRC (2011CB935903), the National Natural Science Foundation of China (20925312), and Shanghai Science Technology Committee (08DZ2270500).
 J.Y. Luo, W.J. Cui, P. He, Y.Y. Xia, Raising the cycling stability of aqueous lithium-ion batteries by eliminating oxygen in the electrolyte, Nature Chemistry 2 (2010) 760.
 J. Yi, X.P. Li, S.J. Hu, W.S. Li, L. Zhou, M.Q. Xu, J.F. Lei, L.S. Hao, Preparation of hierarchical porous carbon and its rate performance as anode of lithium ion battery, Journal of Power Sources 196 (2011) 6670.
 A.R. Armstrong, C. Lyness, P.M. Panchmatia, M.S. Islam, P.G. Bruce, The lithium intercalation process in the low-voltage lithium battery anode Li1 + x V1 − x O2 , Nature Materials 10 (2011) 223.
 N.S. Choi, J.S. Kim, R.Z. Yin, S.S. Kim, Electrochemical properties of lithium vanadium oxide as an anode material for lithium-ion battery, Materials Chemistry and Physics 116 (2009) 603.
 J.H. Song, H.J. Park, K.J. Kim, Y.N. Jo, J.S. Kim, Y.U. Jeong, Y.J. Kim, Electrochemical characteristics of lithium vanadate, Li1 + x VO2 , new anode materials for lithium ion batteries, Journal of Power Sources 195 (2010) 6157.  H.S. Kim, S.O. Kim, Y.T. Kim, J.K. Jung, B.K. Na, J.K. Lee, Electrochemical properties of Li1.1 V0.75 W0.075 Mo0.075 O2 /graphite composite anodes for lithium-ion batteries, Bulletin of Korean Chemical Society 33 (2012) 65.
 W.J. Cui, J. Yi, L. Chen, C.X. Wang, Y.Y. Xia, Synthesis and electrochemical characteristics of NASICON-structured LiSn2 (PO4 )3 anode material for lithium-ion batteries, Journal of Power Sources 217 (2012) 77.
 Z.W. Zhao, Y. Liu, H. Cao, S.J. Gao, M.J. Tu, Phase evolution during synthesis of vanadium carbide (V8 C7 ) nanopowders by thermal processing of the precursor, Vacuum 82 (2008) 852.
 P. Arora, R.E. White, M. Doyle, Capacity fade mechanisms and side reactions in lithium-ion batteries, Journal of the Electrochemical Society 145 (1998) 3647.
 G.N. Zhu, C.X. Wang, Y.Y. Xia, A comprehensive study of effects of carbon coating on Li4 Ti5 O12 anode material for lithium-ion batteries, Journal of the Electrochemical Society 158 (2011) A102.
 M.D. Levi, D. Aurbach, Simultaneous measurements and modeling of the electrochemical impedance and the cyclic voltammetric characteristics of graphite electrodes doped with lithium, Journal of Physical Chemistry B 101 (1997) 4630.
 M.D. Levi, D. Aurbach, Diffusion coefﬁcients of lithium ions during intercalation into graphite derived from the simultaneous measurements and modeling of electrochemical impedance and potentiostatic intermittent titration characstics of thin graphite electrodes, Journal of Physical Chemistry B 101 (1997) 4641.
 D.S. Lu, W.S. Li, X.X. Zuo, Z.Z. Yuan, Q.M. Huang, Study on electrode kinetics of Li+ insertion in Lix Mn2 O4 (0 ≤ x ≤ 1) by electrochemical impedance spectroscopy, Journal of Physical Chemistry C 111 (2007) 12067.
 Y.S. Park, H.J. Bang, S.M. Oh, Y.K. Sun, S.M. Lee, Effect of carbon coating on thermal stability of natural graphite spheres used as anode materials in lithium-ion batteries, Journal of Power Sources 190 (2009) 553.
 Y.T. Lee, C.S. Yoon, J. Prakash, Y.K. Sun, Effect of Li-doping on electrochemical performance of natural graphite anode for lithium secondary batteries, Journal of the Electrochemical Society 151 (2004) A1728.
 Q.M. Pan, K.K. Guo, L.Z. Wang, S.B. Fang, Novel modiﬁed graphite as anode material for lithium-ion batteries, Journal of the Electrochemical Society 149 (2002) A1218.
 H. Yang, H. Bang, K. Amine, J. Prakash, Investigations of the exothermic reactions of natural graphite anode for Li-ion batteries during thermal runaway, Journal of the Electrochemical Society 152 (2005) A73.
 J. Yamaki, H. Takatsuji, T. Kawamura, M. Egashira, Thermal stability of graphite de with electrolyte in lithium-ion cells, Solid State Ionics 148 (2002) 241.